- 1. Crystal Structure Analysis X-ray Diffraction Electron Diffraction Neutron Diffraction Essence of diffraction: Bragg Diffraction Reading: West 5 A/M 5-6 G/S 3 218
- 2. Elements of Modern X-ray Physics, 2nd Ed. by Jens Als-Nielsen and Des McMorrow, John Wiley & Sons, Ltd., 2011 (Modern x-ray physics & new developments) X-ray Diffraction, by B.E. Warren, General Publishing Company, 1969, 1990 (Classic X-ray physics book) Elements of X-ray Diffraction, 3rd Ed., by B.D. Cullity, Addison-Wesley, 2001 (Covers most techniques used in traditional materials characterization) High Resolution X-ray Diffractometry and Topography, by D. Keith Bowen and Brian K. Tanner, Taylor & Francis, Ltd., 1998 (Semiconductors and thin film analysis) Modern Aspects of Small-Angle Scattering, by H. Brumberger, Editor, Kluwer Academic Publishers, 1993 (SAXS techniques) Principles of Protein X-ray Crystallography, 3rd Ed. by Jan Drenth, Springer, 2007 (Crystallography) REFERENCES 219
- 3. SCATTERING Elastic (E’ = E) X-rays scatter by interaction with the electron density of a material. Neutrons are scattered by nuclei and by any magnetic moments in a sample. Electrons are scattered by electric/magnetic fields. Scattering is the process in which waves or particles are forced to deviate from a straight trajectory because of scattering centers in the propagation medium. p' p q E' E h Momentum transfer: Energy change: Inelastic (E’ ≠ E) q 2 sin 2 p Elastic scattering geometry • Rayleigh (λ >> dobject) • Mie (λ ≈ dobject) • Geometric (λ << dobject) • Thompson (X-rays) E pc For X-rays: • Compton (photons + electrons) • Brillouin (photons + quasiparticles) • Raman (photons + molecular vib./rot.)
- 4. COMPTON SCATTERING X-ray source Graphite Target Crystal (selects wavelength) Collimator (selects angle) θ Compton (1923) measured intensity of scattered X-rays from solid target, as function of wavelength for different angles. He won the 1927 Nobel prize. Result: peak in scattered radiation shifts to longer wavelength than source. Amount depends on θ (but not on the target material). A. H. Compton. Phys. Rev. 22, 409 (1923). Detector Compton
- 5. COMPTON SCATTERING Compton’s explanation: “billiard ball” collisions between particles of light (X-ray photons) and electrons in the material Classical picture: oscillating electromagnetic field causes oscillations in positions of charged particles, which re-radiate in all directions at same frequency and wavelength as incident radiation (Thompson scattering). Change in wavelength of scattered light is completely unexpected classically θ e p p Before After Electron Incoming photon p scattered photon scattered electron Oscillating electron Incident light wave Emitted light wave
- 6. Conservation of energy Conservation of momentum 1/2 2 2 2 2 4 e e e h m c h p c m c ˆ e h p i p p 1 cos 1 cos 0 e c h m c 12 Compton wavelength 2.4 10 m c e h m c From this Compton derived the change in wavelength: θ e p p Before After Electron Incoming photon p scattered photon scattered electron COMPTON SCATTERING 223
- 7. Note that there is also an unshifted peak at each angle. Most of this is elastic scatter. Some comes from a collision between the X-ray photon and the nucleus of the atom. 1 cos 0 N h m c N e m m since COMPTON SCATTERING 224 ≈ >>
- 8. COMPTON SCATTERING Contributes to general background noise Diffuse background from Compton emission by gamma rays in a positron emission tomography (PET) scan. 225 Fluorodeoxyglucose (18F)
- 9. X-RAY SCATTERING • wide-angle diffraction (θ > 5°) • small-angle diffraction (θ close to 0°) • X-ray reflectivity (films) elastic (Thompson, ΔE = 0) inelastic (ΔE ≠ 0) • Compton X-ray scattering • resonant inelastic X-ray scattering (RIXS) • X-ray Raman scattering X-rays: • 100 eV (“soft”) – 100 keV (“hard”) photons • 12,400 eV X-rays have wavelengths of 1 Å, somewhat smaller than interatomic distances in solids Diffraction from crystals! First X-ray: 1895 Roentgen 1901 Nobel λ (in Å) = 12400/E (in eV) 226
- 10. DIFFRACTION Diffraction refers to the apparent bending of waves around small objects and the spreading out of waves past small apertures. In our context, diffraction is the scattering of a coherent wave by the atoms in a crystal. A diffraction pattern results from interference of the scattered waves. Refraction is the change in the direction of a wave due to a change in its speed. W. L. Bragg W. H. Bragg diffraction of plane waves von Laue Crystal diffraction I. Real space description (Bragg) II. Momentum (k) space description (von Laue) 227
- 11. OPTICAL INTERFERENCE δ = nλ, n = 0, 1, 2, … δ = nλ, n = 1/2, 3/2, … δ: phase difference n: order perfectly in phase: perfectly out of phase:
- 12. BRAGG’S LAW OF DIFFRACTION When a collimated beam of X-rays strikes pair of parallel lattice planes in a crystal, each atom acts as a scattering center and emits a secondary wave. All of the secondary waves interfere with each other to produce the diffracted beam Bragg provided a simple, intuitive approach to diffraction: • Regard crystal as parallel planes of atoms separated by distance d • Assume specular reflection of X-rays from any given plane → Peaks in the intensity of scattered radiation will occur when rays from successive planes interfere constructively 2Θ 229
- 13. BRAGG’S LAW OF DIFFRACTION AC sin d ACB 2 sin d ACB n 2 sin n d Bragg’s Law: When Bragg’s Law is satisfied, “reflected” beams are in phase and interfere constructively. Specular “reflections” can occur only at these angles. No peak is observed unless the condition for constructive interference (δ = nλ, with n an integer) is precisely met: 230
- 14. DIFFRACTION ORDERS 1st order: 1 2 sin d 2nd order: 2 2 2 sin d By convention, we set the diffraction order = 1 for XRD. For instance, when n=2 (as above), we just halve the d-spacing to make n=1. 2 2 2 sin d 2 2( / 2)sin d e.g. the 2nd order reflection of d100 occurs at same θ as 1st order reflection of d200
- 15. XRD TECHNIQUES AND APPLICATIONS • powder diffraction • single-crystal diffraction • thin film techniques • small-angle diffraction • phase identification • crystal structure determination • radial distribution functions • thin film quality • crystallographic texture • percent crystalline/amorphous • crystal size • residual stress/strain • defect studies • in situ analysis (phase transitions, thermal expansion coefficients, etc) • superlattice structure Uses:
- 16. POWDER X-RAY DIFFRACTION • uses monochromatic radiation, scans angle • sample is powder → all orientations simultaneously presented to beam • some crystals will always be oriented at the various Bragg angles • this results in cones of diffracted radiation • cones will be spotty in coarse samples (those w/ few crystallites) crystallite no restriction on rotational orientation relative to beam 233 2 sin hkl hkl d
- 18. DEBYE-SCHERRER METHOD …or we can use a diffractometer to intercept sections of the cones 235 2 sin hkl hkl d
- 20. General Area Detector Diffraction System (GADDS) DIFFRACTOMETERS
- 21. THIN FILM SCANS 238 4-axis goniometer
- 22. THETA-2THETA GEOMETRY • X-ray tube stationary • sample moves by angle theta, detector by 2theta 239
- 23. THETA-THETA GEOMETRY • sample horizontal (good for loose samples) • tube and detector move simultaneously through theta 240
- 24. POWDER DIFFRACTOGRAMS increasing θ, decreasing d Minimum d? min / 2 d In powder XRD, a finely powdered sample is probed with monochromatic X-rays of a known wavelength in order to evaluate the d-spacings according to Bragg’s Law. Cu Kα radiation: λ = 1.54 Å peak positions depend on: • d-spacings of {hkl} • “systematic absences” 241
- 25. ACTUAL EXAMPLE: PYRITE THIN FILM FeS2 – cubic (a = 5.43 Å) Random crystal orientations On casual inspection, peaks give us d-spacings, unit cell size, crystal symmetry, preferred orientation, crystal size, and impurity phases (none!) 111 200 210 211 220 311 Cu Kα = 1.54 Å 2 Theta Intensity “powder pattern” 2θ = 28.3° → d = 1.54/[2sin(14.15)] = 3.13 Å = d111 reference pattern from ICDD (1,004,568+ datasets)
- 27. 2 theta d 7.2 12.2 14.4 6.1 22 4.0 00 2 sin l d Layered Cuprate Thin film, growth oriented along c axis (hkl) (001) (002) (003) c = 12.2 Å (00l) EXAMPLE 2: textured La2CuO4 Epitaxial film is textured. (It has crystallographic orientation). Many reflections are “missing” 244
- 28. POWDER DIFFRACTION Peak positions determined by size and shape of unit cell Peak intensities determined by the position and atomic number of the various atoms within the unit cell Peak widths determined by instrument parameters, temperature, and crystal size, strain, and imperfections 245 we will return to this later…
- 29. GENERATION OF X-RAYS X-rays beams are usually generated by colliding high-energy electrons with metals. 2p3/2 → 1s Siegbahn notation X-ray emission spectrum
- 31. GENERATION OF X-RAYS Co Kα1 : 1.79 Å Cu Kα1 : 1.54 Å (~8 keV) Mo Kα1 : 0.71 Å / hc h E Side-window Coolidge X-ray tube X-ray energy is determined by anode material, accelerating voltage, and monochromators: 1/2 ( ) C Z Moseley’s Law: 248
- 32. ROTATING ANODES • 100X higher powers possible by spinning the anode at > 6000 rpm to prevent melting it → brighter source 249
- 33. SYNCHROTRON LIGHT SOURCES SOLEIL • brightest X-ray sources • high collimation • tunable energy • pulsed operation GeV electron accelerators 250 Bremsstrahlung (“braking radiation”) Australian Synchrotron
- 34. MONOCHROMATIC X-RAYS Filters (old way) A foil of the next lightest element (Ni in the case of Cu anode) can often be used to absorb the unwanted higher-energy radiation to give a clean Kα beam Crystal Monochromators Use diffraction from a curved crystal (or multilayer) to select X-rays of a specific wavelength 251
- 35. DETECTION OF X-RAYS • Point detectors • Strip detectors • Area detectors Detection principles • gas ionization • scintillation • creation of e-h pairs 252
- 36. DETECTION OF X-RAYS Gas proportional counters Point detectors 253 Scintillation counters
- 37. X-RAY DETECTORS Area detectors Charge-coupled devices • film • imaging plate • CCD • multiwire 254
- 38. X-RAY DETECTORS Imaging plates 255 photostimulated luminescence from BaFBr0.85I0.15:Eu2+
- 39. X-RAY DETECTORS Imaging plates 256 photostimulated luminescence from BaFBr0.85I0.15:Eu2+ tetragonal Matlockite structure (PbFCl) 9-coordinate Ba!
- 40. The Reciprocal Lattice and the Laue Description of Diffraction 257 Reading: A/M 5-6 G/S 3
- 41. PLANE WAVES A wave whose surfaces of constant phase are infinite parallel planes of equal spacing normal to the direction of propagation. ψ: wave amplitude at point r A: max amplitude of wave k: wave vector r: space vector from arbitrary origin k |k|=2π/λ Amplitude is constant in any plane normal to k because k•r is a constant for such planes: k•r1 = kr1 k•r2 = kr1√2(cos45) = kr1 k r2 wavefront origin k r1 45° k•r is indeed constant on wavefronts
- 42. THE RECIPROCAL LATTICE The reciprocal lattice of a Bravais lattice is the set of all vectors K such that for all real lattice position vectors R. 1 i e K R R = n1a1 + n2a2 + n3a3 Direct lattice position vectors: Reciprocal lattice vectors: 2 2 3 1 1 2 3 a a b a a a K = hb1 + kb2 + lb3 2 3 1 2 1 2 3 a a b a a a 2 1 2 3 1 2 3 a a b a a a where the primitive vectors of the reciprocal lattice are: and {ni} and {h,k,l} are integers Reciprocal lattice: The set of all wave vectors K that yield plane waves with the periodicity of a given Bravais lattice. 259
- 43. is satisfied when K•R = 2πn, with n an integer To verify that the {bi} are primitive vectors of the reciprocal lattice, let’s first show that bi•aj = 2πδij 2 2 2 1 2 3 2 3 1 1 1 1 2 3 1 2 3 a a a a a b a a a a a a a a 2 0 3 1 2 1 1 1 2 3 a a b a a a a a 2 0 1 2 3 1 1 1 2 3 a a b a a a a a Indeed, bi•aj = 2πδij so, K•R = (hb1 + kb2 + lb3)•(n1a1 + n2a2 + n3a3) = 2π(hn1 + kn2 + ln3) = 2π × integer (since cross product of two vectors is perpendicular to both) K is indeed a reciprocal lattice vector
- 44. WHAT IS A RECIPROCAL LATTICE VECTOR? The reciprocal lattice is defined at the lattice generated from the set of all vectors K that satisfy for all direct lattice position vectors R. 1 i e K R What is K? a wave vector of a plane wave that has the periodicity of the direct lattice The direct lattice is periodic (invariant under translation by R) Reciprocal lattice vectors = wave vectors of plane waves that are unity at all direct lattice sites 261
- 45. THE RECIPROCAL LATTICE • the reciprocal lattice is defined in terms of a Bravais lattice • the reciprocal lattice is itself one of the 14 Bravais lattices • the reciprocal of the reciprocal lattice is the original direct lattice e.g., simple cubic direct lattice ˆ a 1 a x ˆ a 2 a y ˆ a 3 a z 2 3 2 ˆ ˆ 2 2 a a a 2 3 1 1 2 3 a a b x x a a a 2 ˆ a 2 b y 2 ˆ a 3 b z → simple cubic reciprocal lattice with lattice constant 2π/a → b1 parallel to a1, etc. 262
- 46. Crystals with orthogonal axes (cubic, tetragonal, orthorhombic) b1, b2, b3 are parallel to a1, a2, a3, respectively. b3 a3 b1 a1 a2 b2 reciprocal lattice direct lattice 2 ˆ b 2 b y 2 ˆ a 1 b x 2 ˆ c 3 b z ˆ a 1 a x ˆ b 2 a y ˆ c 3 a z 263
- 47. RECIPROCAL LATTICE OF FCC IS BCC FCC primitive vectors: 2 3 ˆ ˆ ˆ ( ) 4 1 4 ˆ ˆ ˆ 2 2 ( ) 2 (2) 8 a a a 2 3 1 1 2 3 y z - x a a b y z - x a a a Note: not orthogonal 4 1 ˆ ˆ ˆ ( + ) 2 a 2 b z x- y 4 1 ˆ ˆ ˆ ( + ) 2 a 3 b x y - z → BCC reciprocal lattice with lattice constant 4π/a 264
- 48. RECIPROCAL LATTICE OF BCC IS FCC BCC primitive vectors (not orthogonal): 2 3 ˆ ˆ (2 2 ) 4 1 4 ˆ ˆ 2 2 ( ) 2 (4) 8 a a a 2 3 1 1 2 3 y z a a b y z a a a 4 1 ˆ ˆ ( ) 2 a 2 b z + x 4 1 ˆ ˆ ( ) 2 a 3 b x + y → FCC reciprocal lattice with lattice constant 4π/a 265
- 49. RECIPROCAL LATTICES • simple orthorhombic → simple orthorhombic • FCC → BCC • BCC → FCC • simple hexagonal → simple hexagonal (rotated) 266
- 50. = b1 = b2 = b3 β ≠ 90° r. l. d. l. 267
- 51. α,β,γ ≠ 90° 268
- 52. Note that these formulas are missing a factor of 2π 269
- 53. FIRST BRILLOUIN ZONES The Wigner-Seitz cell of the reciprocal lattice is called the first Brillouin zone (FBZ). Wigner-Seitz cell: primitive cell with lattice point at its center enclosed region is W-S cell for 2D hexagonal lattice d.l. FCC r.l. BCC 1st Brillouin zone: truncated octahedron rhombic dodecahedron d.l. BCC r.l. FCC 1st Brillouin zone: 270
- 54. G 000 X (2/a 0 0) L 271
- 55. Brillouin Zone of Diamond and Zincblende Structure (FCC Lattice) • Notation: – Zone Edge or surface : Roman alphabet – Interior of Zone: Greek alphabet – Center of Zone or origin: G 3D BAND STRUCTURE Notation: D<=>[100] direction X<=>BZ edge along [100] direction L<=>[111] direction L<=>BZ edge along [111] direction273
- 56. 274
- 57. Electronic Band Structure of Si <111> <100> <110> Eg 275 Electronic band structure is calculated within the 1st Brilluoin zone
- 58. Theorem: For any family of lattice planes separated by distance d, there are reciprocal lattice vectors perpendicular to the planes, the shortest of which has a length of 2π/d. Conversely, any reciprocal lattice vector K has a family of real-space planes normal to it, separated by d. hk in 2D hkl in 3D here, g = K K and LATTICE PLANES 276 𝐊 = 2𝜋𝑛/𝐝
- 59. Orientation of a plane is determined by its normal vector It is natural to pick the shortest perpendicular reciprocal lattice vector to represent the normal Miller indices: coordinates of this reciprocal lattice vector i.e., A plane with Miller indices hkl is normal to the reciprocal lattice vector K = hb1 + kb2 + lb3 → Definition #2: directions in k-space (Definition #1 was inverse intercepts in the real lattice) MILLER INDICES OF LATTICE PLANES 277
- 60. Proof that K = hb1 + kb2 + lb3 is normal to (hkl) h 1 a AB If K = hb1 + kb2 + lb3 is normal to the plane at left, its dot product with any in-plane vector is zero. Consider vector AB that lies in the plane. By vector addition, l 3 a k 2 a h l AB 3 1 a a The dot product, ( ) h k l h l AB K = 3 1 1 2 3 a a b b b 2 2 0 = So the reciprocal vector formed by using the Miller indices of a plane as its components forms a vector in space that is normal to the Miller plane. Furthermore, the length of the shortest vector K is equal to 2π/dhkl. In the figure above, the spacing between the planes is the projection of : on h K K 1 a 2 2 hkl h d h h K K K K 1 a (hkl) 0 2 hkl K d K → 278 etc.
- 61. REMINDER on ELASTIC SCATTERING p' p q Momentum conservation: q 2 sin 2 p Elastic scattering geometry p p' p elastic scattering: scattering vector
- 62. von LAUE DESCRIPTION OF DIFFRACTION 2 2 sin d n n k 0 2 2 sin k n nK K d • reciprocal space description, equivalent to Bragg description but more powerful for crystallography & solid state physics Equivalence to Bragg picture: K 2 sin 2 sin 2 p q k K q K p k von Laue: “Constructive interference occurs when scattering vector is a reciprocal lattice vector.” since scattering is elastic and ,
- 63. DERIVATION of von LAUE CONDITION Consider two scatterers: Path difference between the rays: ˆ ˆ cos cos ( ) d d ' = ' d n -n Condition for constructive interference: ˆ ˆ ( ) = ' n d n-n Multiply through by 2π/λ: ( - ) = 2 ' n d k k For the Bravais lattice of scatterers: ( - ) = 2 ' n R k k Multiply by i and raise to e: ( - ) 2 = 1 i ' i n e e k k R So, - = ' k k K Diffraction occurs when the change in wave vector, k’-k, is a vector of the reciprocal lattice. 281
- 64. Reciprocal lattice vectors are perpendicular to direct lattice planes Bragg: diffraction when path length difference = nλ Laue: diffraction when scattering vector = recip. vector Alternatively, ' K = k k Laue condition k-space Bragg plane (per. bisector of K) equivalently, when tip of wave vector lies on a k-space Bragg plane 𝐤′ ⋅ 𝐊 = 𝐾2 /2
- 65. EWALD (“e-val”) SPHERE A geometrical construction that provides the relationship between the orientation of a crystal and the direction of the beams diffracted by it. A sphere of radius k centered on the base of the incident wave vector k drawn to the origin O (hkl = 000) of the reciprocal lattice. k k’ θ θ O Projected Ewald sphere (Ewald circle) real space origin of diffraction origin of reciprocal space direction of diffracted beam reciprocal lattice K radius = k ' K = k k Laue condition: (-2,-1) 283
- 66. ' K = k k Laue condition: Diffraction occurs only when a reciprocal lattice point lies on the surface of the Ewald sphere. In this case, hkl = -2,-1,0 so diffraction occurs from the (210) planes and the diffracted beam moves off along k’. -- K k k’ θ θ k k’ θ θ O K (-2,-1) 210 2 / d K = 284
- 67. 285
- 68. In general, a sphere in k-space with the origin on its surface will have no other reciprocal lattice points on its surface: No Bragg peaks for a general incident X-ray! In order to record diffraction patterns, we must either: • use polychromatic radiation (vary the sphere size) → Laue method • rotate the crystal (and thus the reciprocal lattice) → rot. cryst. method • use a powder sample (equivalent to rotating reciprocal space about all angles) → powder method O 286
- 69. 287
- 70. LAUE METHOD • fixed crystal & angle, many wavelengths 288
- 71. The Laue method is mainly used to determine the orientation of large single crystals. When the zone axis lies along the symmetry axis of the crystal, the pattern of Bragg spots will have the same symmetry. 289
- 72. ROTATING CRYSTAL METHOD http://escher.epfl.ch/x-ray/diff.mpeg • single wavelength • aligned crystal is rotated about one axis to rotate reciprocal lattice • produces spots on layer lines k k’ 290
- 73. 291
- 74. POWDER (DEBYE-SCHERRER) METHOD • single wavelength • fixed powder sample • equivalent to rotating the reciprocal lattice through all possible angles about the origin every point in reciprocal space traces out a shell of radius K Each shell with radius K < 2k intersects the Ewald sphere to form a circle. All the diffracted beams from a powder lie on the surface of cones 292
- 75. Peak intensities depend on (in large part): 1) intensity scattered by individual atoms (form factors) 2) the resultant wave from atoms in unit cell (structure factor) PEAK INTENSITIES In many cases, the intensity from certain planes (hkl) is zero. • symmetry of crystal causes complete cancellation of beam “systematic absences” • happenstance Possible reasons: Other factors that affect intensity: • scattering angle • multiplicities • temperature factor • absorption factor • preferred orientation 293
- 76. MONOATOMIC BASES ( - ) 2 = 1 i ' i n e e k k R up to now we have considered diffraction only from Bravais lattices with single atom bases (i.e., atoms only at the lattice points R). We found the diffraction condition: =1 i e K R which is the same as: ( ) i F f e K R K R R K The scattering amplitude FK is the sum over the lattice sites: The scattered intensity is proportional to the absolute square of the amplitude: where fR(K) is the “atomic form factor” for a given atom (disc. later). 2 0 I I F K K …this is what is actually measured in an experiment.
- 77. Crystals with n atoms in each primitive cell must be further analyzed into a set of scatterers at positions d1, d2 … dn within each primitive cell. ( ) ( ) j i j j F f e K R+d K R K n-ATOM BASES ( ) j j A R R d The positions of the atoms are: making the scattering amplitude: ( ) j i i j j e f e K d K R R K i L e K R R ( ) j i j j f e K d K K “Lattice sum” “Structure factor” of the basis *If the structure factor = 0, there is no diffraction peak.
- 78. ( ) j i j j f e K d K K The structure factor gives the amplitude of a scattered wave arising from the atoms with a single primitive cell. STRUCTURE FACTOR For crystals composed of only one type of atom, it’s common to split the structure factor into two parts: ( ) j f S K K K j i j S e K d K “atomic form factor” “geometric structure factor” S = 0 gives a systematic absence (i.e., absence of expected diff. peak). 296
- 79. 2 ( ) hkl I S K 1 i e K d n i e K d … 1 j n i j S e K K d The amplitude of the rays scattered at positions d1, …, dn are in the ratios: The net ray scattered by the entire cell is the sum of the individual rays: STRUCTURE FACTORS Geometric structure factor -Adds up scattered waves from unit cell -In particular, no peak when SK = 0 297
- 80. For simple cubic: one atom basis (0,0,0) 0 1 i S e K K SIMPLE CUBIC d1 = 0a1 + 0a2 + 0a3 298 Same result as simple monatomic basis
- 81. For monoatomic BCC: we can think of this as SC with two point basis (0,0,0), (½,½,½) l k h ) 1 ( 1 S = 2, when h + k + l even S = 0, when h + k + l odd (systematic absences) 2 ( ) 0 2 1 ( ) 1 j a i x y z i i j i h k l S e e e e K K K K d MONATOMIC BCC 2 ˆ ˆ ˆ ( ) h k l a K x y z For SC, 299
- 82. e.g. consider the powder pattern of BCC molybdenum Powder card shows only even hkl sums b/c Mo is BCC Why? - Diffraction from other (hkl) results in destructive interference: (100) d100 Beam cancels b/c body center atoms scatter exactly 180° out of phase (200) d200 Strong reflection b/c all atoms lie on 200 planes and scatter in phase
- 83. S = 4 when h + k, k + l, h + l all even (h, k, l all even or all odd) S = 0 otherwise. ( ) ( ) ( ) 1 i h k i k l i h l S e e e K For monoatomic FCC: SC with four point basis (0,0,0), (½,½,0), (0,½,½), (½,0,½) 4 ( ) ( ) ( ) 0 2 2 2 1 j a a a i x y i y z i x z i i j S e e e e e K K K K K K d MONATOMIC FCC 2 ˆ ˆ ˆ ( ) h k l a K x y z For SC, 301
- 84. POLYATOMIC STRUCTURES Atoms of different Z in the unit cell have different scattering powers, so we explicitly include the form factors: Total structure factor {fj }: atomic form factors # of electrons ( ) j i j j f e K d K K 302
- 85. Cesium Chloride is primitive cubic Cs (0,0,0) Cl (1/2,1/2,1/2) but what about CsI? ( ) i h k l Cs Cl f f e K CsCl STRUCTURE Cs+ and Cl- are not isoelectronic → systematic absences unlikely ( ) j i j j f e K d K K 303 Φ = f Cs + fCl when h + k + l even Φ = f Cs - fCl when h + k + l odd
- 86. (hkl) CsCl CsI (100) (110) (111) (200) (210) (211) (220) (221) (300) (310) (311) Cs+ and I- are isoelectronic, so CsI looks like BCC lattice: 304 h + k + l even
- 87. Diatomic FCC Lattices Sodium Chloride (NaCl) Na: (0,0,0)(0,1/2,1/2)(1/2,0,1/2)(1/2,1/2,0) Cl: (1/2,1/2,1/2) (1/2,1,1)(1,1/2,1)(1,1,1/2) Add (1/2,1/2,1/2) 305
- 88. Φ = 4(fNa + fCl) when h, k, l, all even Φ = 4(fNa - fCl) when h, k, l all odd Φ = 0 otherwise ( ) , [ ][ ] i h k l Na Cl FCC f f e S K K 306 ( ) ( ) ( ) ( ) [ ][1 ] i h k l i h k i h l i l k Na Cl f f e e e e K
- 89. (hkl) NaCl KCl (100) (110) (111) (200) (210) (211) (220) (221) (300) (310) (311) Once again, there are more systematic absences for isoelectronic ions (e.g., K and Cl) (110) always absent in RS (111) sometimes absent 307
- 90. For RS, we expect the intensity of the all odd reflections to increase with increasing ΔZ between cation and anion: I111,311 : KCl < KF < KBr < KI Less complete destructive interference between cation and anion sublattices. 308
- 91. DIAMOND STRUCTURE Diamond: FCC lattice with two-atom basis (0,0,0,), (¼,¼,¼) ( ) 0 4 , , ( /2)( ) , [ ][ ] [1 ][ ] a iK x y z iK diamond FCC i h k l FCC S e e S e S K K K S = 8 h + k + l twice an even number S = 4(1 ± i) h + k + l odd S = 0 h + k + l twice an odd number IFCC : all nonvanishing spots have equal intensity. Idiamond : spots allowed by FCC have relative intensities of 64, 32, or 0. 309 Only for all even or all odd hkl is S ≠ 0. For these unmixed values, Additional condition:
- 92. (hkl) Al Si (100) (110) (111) (200) (210) (211) (220) (221) (300) (310) (311) What about zinc blende? FCC diamond 310
- 93. SUMMARY OF SYSTEMATIC ABSENCES crystal structure condition for peak to occur SC any h,k,l BCC h + k + l = even FCC h,k,l all even or all odd NaCl h,k,l all even, or all odd if fA ≠ fB diamond h,k,l all even and twice an even #, or all odd HCP any h,k,l except when h + 2k = 3n and l is odd ( ) j i j j f e K d K K 311
- 94. Observable diffraction peaks for monoatomic crystals 2 2 2 l k h SC: 1,2,3,4,5,6,8,9,10,11,12,… BCC: 2,4,6,8,10,12,... FCC: 3,4,8,11,12,16,24,… SIMPLE ANALYSIS OF SIMPLE PATTERNS What will we see in XRD patterns of SC, BCC, FCC? SC FCC BCC We can take ratios of (h2 + k2 + l2) to determine structure.
- 95. SIMPLE ANALYSIS OF SIMPLE PATTERNS n d sin 2 2 2 2 l k h a dhkl For cubic crystals: 2 2 1 sin hkl d 2 2 2 2 sin ( ) h k l 2 2 2 2 th peak th peak 2 2 2 2 1st peak 1st peak sin ( ) sin ( ) n n h k l h k l 313
- 96. 2 2 2 2 2 1 sin sin 33 2 sin sin 22 SIMPLE ANALYSIS OF SIMPLE PATTERNS 110 200 211 α-Fe is cubic. Is it FCC or BCC? BCC! What about Al? 2 2 2 2 2 1 sin sin 22.5 1.33 sin sin 19 111 200 220 311 222 400 331 420 FCC! 314
- 97. Ex: An element, BCC or FCC, shows diffraction peaks at 2: 40, 58, 73, 86.8,100.4 and 114.7. Determine:(a) Crystal structure?(b) Lattice constant? (c) What is the element? 2theta theta (hkl) 40 20 0.117 1 (110) 58 29 0.235 2 (200) 73 36.5 0.3538 3 (211) 86.8 43.4 0.4721 4 (220) 100.4 50.2 0.5903 5 (310) 114.7 57.35 0.7090 6 (222) 2 sin 2 2 2 l k h BCC, a =3.18 Å W normalized 315
- 98. ELASTIC X-RAY SCATTERING BY ATOMS Atoms scatter X-rays because the oscillating electric field of an X-ray sets each electron in an atom into vibration. Each vibrating electron acts as a secondary point source of coherent X-rays (in elastic scattering). Thomson relation: The X-ray scattered from an atom is the resultant wave from all its electrons Particle picture: • zero phase difference for forward/backward scattering → scattering factor (form factor, f ) proportional to atomic number, Z • increasingly destructive interference with larger scattering angle (to 90°) • for a given angle, intensity decreases with decreasing X-ray wavelength • max scattering intensity at 2θ = 0 & 180° • gradual decrease to 50% as 2θ approaches 90° 2 1 (1 cos 2 ) 2 I
- 99. SCATTERING OF X-RAYS BY ATOMS Thomson relation: 2 1 (1 cos 2 ) 2 I scattering angle probabilities for a free electron: Low energy: Thomson High energy: Compton Klein–Nishina formula
- 100. ATOMIC FORM FACTORS Form factor f = scattering amplitude of a wave by an isolated atom • Z (# electrons) • scattering angle • X-ray wavelength For X-rays, f depends on: consequences: • powder patterns show weak lines at large 2θ. • light atoms scatter weakly and are difficult to see. 0 ( ) ( ) i j j f e d q r q r r 4 sin q with, For θ = 0 (forward scattering), scattering vector q General elastic formula: 0 (0) ( ) j f d # electrons r r = O K+ Cl- Cl θ = 37° 3 3
- 101. ELECTRON DENSITY MAPS The electron density as a function of position x,y,z is the inverse Fourier transform of the structure factors: The electron density map describes the contents of the unit cells averaged over the whole crystal (not the contents of a single unit cell) 2 ( ) 1 ( ) i hx ky lz hkl hkl xyz e V 319
- 102. PEAK WIDTHS Peak shape is a Voigt function (mixture of Gaussian and Lorentzian) Peak width (broadening) is determined by several factors: • natural linewidth of X-ray emission • instrumental effects (polychromatic λ, focusing, detector) • specimen effects 1) crystallite size 2) crystallite strain • Gaussian component arises from natural linewidth and strain • Lorentzian component arises from coherent domain size Pure Lorentzian Pure Gaussian 320
- 103. 321 FULL WIDTH AT HALF MAXIMUM (FWHM) Can also be fit with Gaussian, Lorentzian, Gaussian-Lorentzian etc.
- 104. Instrument and Sample Contributions to the Peak Profile must be Deconvoluted • In order to analyze crystallite size, we must deconvolute: – Instrumental Broadening FW(I) • also referred to as the Instrumental Profile, Instrumental FWHM Curve, Instrumental Peak Profile – Specimen Broadening FW(S) • also referred to as the Sample Profile, Specimen Profile • We must then separate the different contributions to specimen broadening – Crystallite size and microstrain broadening of diffraction peaks 322
- 105. SIZE BROADENING Small crystallites (< 200 nm) show broadened diffraction lines Nanocrystal X-ray Diffraction 323
- 106. 324
- 107. Which of these diffraction patterns comes from a nanocrystalline material? 66 67 68 69 70 71 72 73 74 2(deg.) Intensity (a.u.) These diffraction patterns were produced from the same sample! • Two different diffractometers, with different optical configurations, were used • The apparent peak broadening is due solely to the instrumentation in this case 325
- 108. 1 2 3 4 j-1 j j+1 2j-1 2j B 1 2 at Bragg angle, phase lag between two planes = perfectly in phase, constructive B B 1 At some angle Phase lag between two planes: At (j+1)th plane: Phase lag: • Rays from planes 1 and j+1 cancel • Ditto for 2 & j+2, … j & 2j • Net diffraction over 2j planes = 0 2 j The finite size of real crystals results in incomplete destructive interference over some range of angles Crystal with 2j planes Total thickness T T = (2j-1)d The angular range θB to θ1 is the range where diffracted intensity falls from a maximum to zero (half of Bragg peak profile).
- 109. Same arguments apply to B 2 So we see diffracted X-rays over all scattering angles between 2θ1 and 2θ2. – If we assume a triangular shape for the peak, the full width at half maximum of the peak will be B = (2θ1 – 2θ2)/2 = θ1 – θ2 327
- 110. If we have more than 2j planes: 1 2 3 4 j-1 j j+1 2j+1 2j+2 B 1 2 If we have fewer than 2j planes: 1 2 3 4 j-1 j j+1 2j-3 2j-2 B 1 2 still zero intensity at θ1 nonzero intensity at θ1 Rays from planes j-1 & j not canceled Rays from new planes are canceled Thinner crystals result in broader peaks! 328 Peak sharpens! Peak broadens!
- 111. Let’s derive the relation between crystal thickness T and peak width B: 2 sin d 1 2 2 sin (2 1) 2 sin (2 1) T j T j 1 2 (sin sin ) T 1 2 1 2 2 (cos( )sin( )) 2 2 T 1 2 2 (cos )( )) . 2 B T cos B T B 1 2 2( ) 2 B Considering the path length differences between X-rays scattered from the front and back planes of a crystal with 2j+1 planes and total thickness T: If we subtract them: Using trig identity: Since and , 1 2 2 B 1 2 1 2 sin( ) 2 2 But, , so 1 2 1 2 1 2 sin sin 2cos sin 2 2 Here, T = 2jd
- 112. cos B K T B 2 2 2 M R B B B BM: Measured FWHM (in radians) BR: Corresponding FWHM of bulk reference (large grain size, > 200 nm) Readily applied for crystal size of 2-100 nm. Up to 500 nm if synchrotron is used. SCHERRER FORMULA A more rigorous treatment includes a unitless shape factor: Scherrer Formula (1918) T = crystallite thickness λ (X-ray wavelength, Å) K (shape factor) ~ 0.9 B, θB in radians Accurate size analysis requires correction for instrument broadening: 330 For Gaussian peaks:
- 113. • The constant of proportionality, K (the Scherrer constant) depends on the how the width is determined, the shape of the crystal, and the size distribution – the most common values for K are: • 0.94 for FWHM of spherical crystals with cubic symmetry • 0.89 for integral breadth of spherical crystals w/ cubic symmetry • 1, because 0.94 and 0.89 both round up to 1 – K actually varies from 0.62 to 2.08 • For an excellent discussion of K, refer to JI Langford and AJC Wilson, “Scherrer after sixty years: A survey and some new results in the determination of crystallite size,” J. Appl. Cryst. 11 (1978) 102-113. cos B K T B SCHERRER CONSTANT 0.94 cos B T B 331
- 114. Suppose =1.5 Å, d=1.0 Å, and =49°. Then for a crystal 1 mm in diameter, the width B, due to the small crystal effect alone, would be about 2x10-7 radian (10-5 degree), too small to be observable. Such a crystal would contain some 107 parallel lattice planes of the spacing assumed above. However, if the crystal were only 50 Å thick, it would contain only 51 planes, and the diffraction curve would be very broad, namely about 43x10-2 radian (2.46°), which is easily measurable. 332 “Incomplete destructive interference at angles slightly off the Bragg angles”
- 115. What do we mean by crystallite size? “A single-crystalline domain that scatters coherently” • A particle may be made up of several different crystallites (also called grains) • The crystallites, not the particles, are the coherent scattering units 333
- 116. • Though the shape of crystallites is usually irregular, we can often approximate them as: – sphere, cube, tetrahedra, or octahedra – parallelepipeds such as needles or plates – prisms or cylinders • Most applications of Scherrer analysis assume spherical crystallite shapes • If we know the average crystallite shape from another analysis, we can select the proper value for the Scherrer constant K • Anisotropic crystal shapes can be identified by unequal peak broadening – if the dimensions of a crystallite are 2x * 2y * 200z, then (h00) and (0k0) peaks will be more broadened than (00l) peaks. CRYSTALLITE SHAPE 334 e.g., a nanowire
- 119. Non-Uniform Lattice Distortions • Rather than a single d-spacing, the crystallographic plane has a distribution of d-spacings • This produces a broader observed diffraction peak • Such distortions can be introduced by: – mechanical force – surface tension of nanocrystals – morphology of crystal shape, such as nanotubes – interstitial impurities 26.5 27.0 27.5 28.0 28.5 29.0 29.5 30.0 2 (deg.) Intensity (a.u.) 337
- 120. THIN FILM SCANS 338
- 121. 339
- 122. 340 EPITAXY - “above in an ordered fashion” when one crystal grows on another with a well-defined 3D crystallographic relationship Homoepitaxy: epitaxy between identical crystals (e.g., Si on Si) Heteroepitaxy: the two crystals are different (e.g., ZnO on Al2O3) requirements: lattice symmetry & lattice constant matching
- 123. 341 Dan Connelly Molecular picture – Si growth on Si (100)
- 124. 342 NTNU
- 125. 343 Rock salt PbS “nanotrees” Jin group – U. Wisc. branches grow epitaxially – each tree is a single crystal
- 126. A polycrystalline sample should contain thousands of crystallites. Therefore, all possible diffraction peaks should be observed. 2 2 2 • For every set of planes, there will be a small percentage of crystallites that are properly oriented to diffract (the plane perpendicular bisects the incident and diffracted beams). • Basic assumptions of powder diffraction are that for every set of planes there is an equal number of crystallites that will diffract and that there is a statistically relevant number of crystallites, not just one or two. 344
- 127. A single crystal specimen in a Bragg-Brentano diffractometer would produce only one family of peaks in the diffraction pattern. 2 At 20.6 °2, Bragg’s law fulfilled for the (100) planes, producing a diffraction peak. The (110) planes would diffract at 29.3 °2; however, they are not properly aligned to produce a diffraction peak (the perpendicular to those planes does not bisect the incident and diffracted beams). Only background is observed. The (200) planes are parallel to the (100) planes. Therefore, they also diffract for this crystal. Since d200 is ½ d100, they appear at 42 °2. 345
- 128. Wurtzite ZnO nanowire arrays on glass Good uniaxial texture Poor uniaxial texture Biaxial texture (growth on Al2O3) c 346 General route to vertical ZnO nanowire arrays using textured ZnO seeds. Greene, L. E., Law, M., Tan, D. H., Montano, M., Goldberger, J., Somorjai, G., Yang, P. Nano Letters 5, 1231-1236 (2005).
- 129. ROCKING CURVES 347
- 130. ROCKING CURVES 348
- 131. ROCKING CURVE EXAMPLES Thickness, composition, and strain state of epitaxial single crystal films
- 132. ROCKING CURVE EXAMPLE Thickness, composition, and strain state of epitaxial single crystal films 350 (1° = 3600 arcsec)
- 133. 351 sit on a reflection, then rotate in-plane PHI SCANS
- 134. 352 k-SPACE GEOMETRY for rotation around [001] of cubic crystal: monitor {011}: expect 4 peaks separated by 90° rotation. monitor {111}: expect 4 peaks separated by 90° rotation. (ignoring possible systematic absences) two examples:
- 135. PHI SCAN EXAMPLE 1 um GaN (wurtzite) on Silicon(111) 2-theta scan proves uni-axial texture phi scan proves bi-axial texture (epitaxy) (002) (1011) In plane alignment: GaN[1120]//Si[110] 353
- 136. Epitaxial YBa2Cu3O7 on Biaxially Textured Nickel (001): An Approach to Superconducting Tapes with High Critical Current Density Science, Vol 274, Issue 5288, 755-757 , 1 November 1996 354
- 137. Epitaxial YBa2Cu3O7 on Biaxially Textured Nickel (001): An Approach to Superconducting Tapes with High Critical Current Density Science, Vol 274, Issue 5288, 755-757 , 1 November 1996 omega phi 355
- 138. TEXTURE MEASUREMENT (POLE FIGURES) ψ 356
- 139. stereograms showing all poles of a particular hkl plane, with axes defined by an external frame of reference. – pole figures map the intensity of a single hkl as a function of tilt and rotation of the sample – most common way to map crystallographic texture POLE FIGURES 357 e.g., a textured polycrystalline rolled metal sheet: untextured sheet textured sheet
- 140. Example: c-axis aligned superconducting thin films. (b) (a) Biaxial Texture (105 planes) Random in-plane alignment POLE FIGURE EXAMPLE – PHI ONLY 358
- 141. SMALL ANGLE X-RAY SCATTERING 359
- 142. SAXS: diffraction from planes with > 1 nm d-spacing 360
- 143. Direct Visualization of Individual Cylindrical and Spherical Supramolecular Dendrimers Science 17 October 1997; 278: 449-452 Small Angle X-ray Diffraction 361
- 144. Triblock Copolymer Syntheses of Mesoporous Silica with Periodic 50 to 300 Angstrom Pores Science, Vol 279, Issue 5350, 548-552 , 23 January 1998 362 HCP
- 145. 363 GRAZING INCIDENCE SAXS (GISAXS)
- 147. Rigaku SmartLab XRD 0D, 1D, 2D detectors In-plane & Out-of-plane Thin-film XRD High resolution XRD SAXS μ-XRD Capillary transmission 1500°C heating stage 1100°C dome stage UCI XRD
- 148. 366
- 150. Why ED patterns have so many spots λX-ray = hc/E = 0.154 nm @ 8 keV λe- = h/[2m0eV(1 + eV/2m0c2)]1/2 = 0.0037 nm @ 100 keV Typically, in X-ray or neutron diffraction only one reciprocal lattice point is on the surface of the Ewald sphere at one time. In electron diffraction the Ewald sphere is not highly curved b/c of the very short wavelength electrons that are used. This nearly-flat Ewald sphere intersects with many reciprocal lattice points at once. - In real crystals reciprocal lattice points are not infinitely small and in a real microscope the Ewald sphere is not infinitely thin 368
- 151. DIFFRACTION FROM DISORDERED SOLIDS amorphous solids 369
- 152. Index planes Calculate crystal density Calculate d-spacings Derive/use Bragg’s Law Index diffraction peaks Determine lattice constants Reciprocal lattice Ewald sphere construction Calculate structural factors, predicting X-ray diffraction pattern (systematic absences) Use of Scherrer relation DIFFRACTION: WHAT YOU SHOULD KNOW 370
- 153. Term Paper and Presentation Choose a contemporary materials topic that interests you. For example: • Organic LEDs • Metamaterials • Multiferroics • Graphene • Photonic Crystals • Amorphous Metals • Colossal Magnetoresistance • Synthetic Biomaterials • Infrared Photodetectors • Conducting Polymers • Inorganic Solar Cells • Plasmonics • High κ Dielectrics • Quantum Dots 1) Quantitatively explain the basic principles at work 2) Summarize the state-of-the-art in synthesis, properties, and apps 3) Identify a key challenge facing the field and propose an original solution to this challenge In ≥10 pages of double-spaced text (+ figures and references): 371
- 154. Term Paper Due Dates February 24: Topic selection. E-mail me with a one-paragraph abstract describing your topic, challenge, and proposed solution 372 8-10 am March 20: Paper submission and 5-minute presentation to educate the class on your topic.
- 155. Midterm Exam • February 19 • full class period • short answer questions • topics up through the end of diffraction • calculator, pens, pencils, nothing else • focused on conceptual understanding, not memorization 373 (b) 4 pts. The graph below shows a single Bragg reflection from a powder sample of large crystallites. On the same graph, sketch the peak expected for a sample of this solid consisting of small crystals under substantial uniform compressive stress. 2 theta intensity Peak will be broader and shifted to higher 2θ (smaller d-spacing)